Responsive plasma polymerized ultrathin nanocomposite · PDF file Responsive plasma...
Embed Size (px)
Transcript of Responsive plasma polymerized ultrathin nanocomposite · PDF file Responsive plasma...
at SciVerse ScienceDirect
Polymer 53 (2012) 4686e4693
Contents lists available
journal homepage: www.elsevier .com/locate/polymer
Responsive plasma polymerized ultrathin nanocomposite films
Kyle D. Anderson a, Robert B. Weber a, Michael E. McConney b, Hao Jiang b, Timothy J. Bunning b, Vladimir V. Tsukruk a,* a School of Materials Science and Engineering, Georgia Institute of Technology, Atlanta, GA 30332, United States bMaterials and Manufacturing Directorate, Air Force Research Laboratory, Wright-Patterson Air Force Base, Dayton, OH 45433-7702, United States
a r t i c l e i n f o
Article history: Received 28 May 2012 Received in revised form 27 July 2012 Accepted 4 August 2012 Available online 21 August 2012
Keywords: NIPAAM Plasma polymerization Co-polymerization Responsive films Tunable optical properties
* Corresponding author. Tel.: þ1 404 894 6081; fax E-mail address: firstname.lastname@example.org (V.V. Ts
0032-3861/$ e see front matter � 2012 Elsevier Ltd. http://dx.doi.org/10.1016/j.polymer.2012.08.013
a b s t r a c t
The plasma polymerization of NIPAAM and titanium isopropoxide monomers into responsive ultrathin films with responsive optical properties using plasma enhanced chemical vapor deposition is reported. The composite ultrathin films possess a large window for potential changes in their refractive index from 1.60 to 1.95. We demonstrated that these polymer films exhibit fast (transition time below 2 s), large, reversible, and repeatable changes to their thickness and refractive index as a function of periodic environmental humidity changes.
� 2012 Elsevier Ltd. All rights reserved.
Material coatings capable of autonomous, self-actuating response to specific stimuli are desirable in a wide range of applications including thermalandchemical sensing, tunableoptics, targeteddrug delivery, switchable surfaces and micro actuators [1e6]. Designing materials which are capable of generating a response from the stim- ulus itself eliminates the need for additional and complex triggering and control mechanisms as the response process will be fully con- tained within a layer of material integrated into the larger system. Responsive ultrathinpolymeric films have been utilized in an array of applications through a variety of synthesis methods and materials. Polymers including poly(N-isopropylacrylamide) (pNIPAAM) exhibit a large response to temperature in a fluid environment, typically as a change in thickness for thin films, under appropriate conditions as has been widely reported [7e11]. Recent examples include coatings fabricated with UV-photografting and chemical vapor deposition (CVD) techniques [12e16]. This type of switching behavior can be used to drive mechanical changes in systems, actuate folding behavior, alter surface mechanical properties or enhance switchable cell scaffoldings [17e20].
Plasma enhanced chemical vapor deposition (PECVD) poly- merization is a unique thin film fabrication method which allows
: þ1 404 385 3112. ukruk).
All rights reserved.
the direct deposition and polymerization of a wide variety of monomers directly on a target substrate through a one step, robust, solvent-less deposition process [21,22]. PECVD typically utilizes an RF plasma in a low pressure argon atmosphere to radicalize monomer vapor in the plasma stream. PECVD helps to overcome limitations in wet chemical surface modification including chal- lenges with grafting and polymerization while providing a method to precisely control the optical properties of the deposited film. Similar to other CVD techniques, this variant has been utilized for use with organic monomers to enable the formation of a variety of atypical polymers deposited directly onto various planar, freely suspending, and textured substrates for numerous surface modifi- cation applications [23e28]. The range of precursors has covered many traditional reactive monomers such as styrene, ethylene glycol and benzene, as well as responsive materials like 2- hydroxyethyl methacrylate, 2-vinylpyridine and N-iso- propylacrylamide and biological monomers such as amino acids [29e35]. PECVD allows deposition under “dry” conditions meaning that only the puremonomer and no additional solvents, surfactants or reactants are needed in the synthesis of the film. This approach becomes especially useful for the fabrication of robust coatings which may otherwise require complex wet chemical procedures to firmly attach to some surfaces.
A number of recent studies have exploited pNIPAAM as a plasma polymerizable material which retains its well-known and charac- teristic temperature and humidity response properties [12,33,34].
Delta:1_given name Delta:1_given name Delta:1_surname Delta:1_given name Delta:1_given name Delta:1_surname Delta:1_given name Delta:1_given name Delta:1_surname Delta:1_given name Delta:1_given name Delta:1_surname mailto:email@example.com www.sciencedirect.com/science/journal/00323861 http://www.elsevier.com/locate/polymer http://dx.doi.org/10.1016/j.polymer.2012.08.013 http://dx.doi.org/10.1016/j.polymer.2012.08.013 http://dx.doi.org/10.1016/j.polymer.2012.08.013
Scheme 1. NIPAAM (left) and TTIP (right) monomers used in plasma polymerizations.
Fig. 1. AFM of A, B) PP-NIPAAM (Z ¼ 2 nm), C, D) PP-TTIP (Z ¼ 16 nm), E, F) P
K.D. Anderson et al. / Polymer 53 (2012) 4686e4693 4687
Hess et al. conducted extensive temperature and pressure experi- ments and related changes of the crosslinking properties as measured via FTIR and contact angle measurements back to the reactor conditions . These observations indicate a similar low critical solution temperature (LCST) phase transition and swelling properties of these plasma polymerized materials to bulk materials . Ratner et al. investigated the LCST effects in plasma poly- merized NIPAAM using AFM mechanical data measurements as a function of temperature [12,36]. Gleason et al. recently demon- strated the ability to control the LCST between 16 and 28 �C . This was achieved by varying the amount of co-monomer
P-NIPAAM/TTIP (Z ¼ 14 nm) at low (left) and high (right) magnifications.
3500 3000 2500 2000 1500
3500 3000 2500 2000 1500
3500 3000 2500 2000 1500 1000 500
3500 3000 2500 2000 1500 1000 500
3500 3000 2500 2000 1500
pNIPAAM A B
Fig. 2. FTIR spectra of A) NIPAAM monomer B) Spun-cast P-NIPAAM film and plasma polymerized films: C) PP-NIAAM, D) PP-TTIP and E) PP-NIPAAM/TTIP.
K.D. Anderson et al. / Polymer 53 (2012) 4686e46934688
polymerized with the NIPAAM during initiated CVD. These films showed a similar response to other reports, providing further evidence that NIPAAM thin films can be used in rapid responsive microactuator or MEMS devices. Overall, these plasma polymerized films with relatively high crosslinking density show modest response in comparison with bulk gels . Several recent studies have evaluated co-polymerization of distinct monomers for significant refractive index modification [39,40]. The addition of two or more monomers, each with a distinctive refractive index,
can be used as a method to create films with precisely tuned refractive indices set at a desired value [41,42]. Additionally, optical stacks have been fabricated which show remarkable tunablility with a significant shift in reflectivity properties upon activation using swellable hydrogels sandwiched between high index layers .
Here, we demonstrate robust plasma polymerized single compo- nentfilms of NIPAAMand Titanium(IV) isopropoxide (TTIP) aswell as corresponding robust compositefilms from these components. These
Table 1 FTIR peak assignments for plasma polymerized films.
NIPAAM pNIP AAM
PP-TTIP PP-NIPAAM/ TTIP
NeH stretch 3298 3275 3272 3272 OeH stretch 3252 CeH stretch 2969 2974 2973 2973 C]O stretch (amide I) 1657 1640 1645 1646 CeC stretch 1622 1628 NeH stretch (amide II) 1548 1548 1547 1548 CeH symmetric bending 1454 1462 1463 1454 CeCH3 methyl bending I 1387 1389 1390 1384 CeCH3 methyl bending II 1367 1368 1366 1376 TieO 699 697
K.D. Anderson et al. / Polymer 53 (2012) 4686e4693 4689
ultrathin composite films exhibiting a wide range of controllable refractive indices and, moreover, this refractive index responds significantly and reversibly to periodic environment humidity changes with much faster response time than that usually observed for traditional bulk one-component PNIPAAM films.
All monomers, N-Isopropylacrylamide (97%) and titanium(IV) isopropoxide (99%) were purchased from SigmaeAldrich and used as received for all subsequent plasma processes (Scheme 1). All plasma depositions were carried o